changing technology ln a changing world - fathi...changing technology ln a changing world the case...
Post on 19-Aug-2018
Embed Size (px)
CHANGING TECHNOLOGY lN A CHANGING WORLD
THE CASE OF EXTRACTIVE METALLURGY 1
Smelting of ores for metal extraction is an ancient art in our civilization. New technology is being introduced, but forces of resistance are sometimes so strong to permit a radical change. While the iron and steel, zinc, aluminum, and gold industries are responding to change, the copper and nickel industries seem to be more conservative.
Key words: iron, steel, copper, pressure hydrometallurgy, gold, alurninum, zinc, nickel, sulfur dioxide, elemental sulfur, sulfuric acid, pyrite, arsenopyrite.
' XVII Encontro Nacional de Tratamento de Minrios e Metalurgia Extrativa - I Simpsio sobre Qumica de Colides- Aguas de Sao Pedro- SP, Brazil , August 23-26. 1998. : Department of Mining and Metallurgy, Lavai University, Qut:bec City, Canada
Extractive metallurgy today is usually divided in two sectors: ferrous and nonferrous because of the large scale operations in the ferrous [1). Steel production in one year exceeds that of ali other metais combined in ten years. As a result, metallurgists in the nonferrous sector usually do not participate in the activities of iron and steel makers and vice versa. This is a pity because for sure one can leam from the other. ln fact, the copper industry adopted many technologies used first in iron and steel production. For example, when Bessemer invented the conventer in 1856 it was adopted in the copper industry ten years !ater, and when high grade massive copper sulfide ores were exhausted and metallurgists were obliged to treat low-grade ores, the puddling furnace was adapted in form of a reverberatory furnace to treat the flotation concentrates. Continuous casting started first in steel plants and was adopted !ater in the nonferrous industry. ln general, the copper industry was in the footsteps of the iron industry although the two chemistries are far apart.
Pyrometallurgy is an ancient art and is most suitable for treating high grade oxide ores [2). It is beyond doubt that iron will always be produced by pyrometallurgical route since iron occurs in nature mainly as an oxide. The case of copper is, however, different. But, before discussing the copper situation it will be interesting to review the changing technology in iron and steel production.
The reduction of iron ore to produce metallic iron took place in ancient times in a smal! fumace 2 to 3 meters high, charged with lumps of iron ore mixed with pieces of charcoal prepared from timber. Air required for buming of charcoal to supply the necessary heat for reduction was supplied by small bellows. The ore lumps were reduced to iron but not melted because the air draft was not strong enough to generate the high temperature needed for melting. When the fumace was cooled, the lump of metallic iron mixed with partially melted gangue minerais and slag, is then removed from the fumace, heated and hammered to get a consolidated metallic product. A fumace of this type would produce I or 2 kilograms of malleable iron per day which was enough to supply the need of that time(Figure 1).
The large charcoal furnace
To increase productivity, large fumaces were built with large air bellows mechanically operated by large water wheels. As a result, the temperature increased, and the iron produced melted in the furnace. Some iron was tapped directly into moulds in the casting house and the remaining was collected by allowing it to drain into sand moulds (called "pigs") prepared in the immediate vicinity. The product contained much dissolved carbon and was suitable for casting many items. A furnace of this period would be 5 to 10 meters high and would produce 10 or 20 tons of iron per day. The maximum size of the fumace was limite,d by the mechl!Ilical strength of the charcoal. To produce a high quality iron for tools and knives, it was necessary to refine this cast iron in what was known as a "finery". Small pieces of the
cast iron were remelted in an oxidizing atmosphere to remove as much as possible of the carbon (Figure 2) .
AIRBLOWN BY SMALL BELLOWS
II.C0.4 (wroughl iron & slag)
WRO..GHT R:lN Carbonfree iron
Figure 1 - Production of wrought iron in a short charcoal fumace with small air bellows.
CHARCOAL IAON ORE
AIRBLOWN BYLARGE BELLOWS
CAST IRON tro n conta in1ng
24 % carbon
Figure 2 - Production of cast iron in a short charcoal fumace with Jarge air bellows.
The coke furnace
The industrial revolution startoo in England in 1709 when charcoal was substituted by coke. Coke is produced from coai - - it is porous and can withstand high mechanical pressures . Hence larger fumaces could be built which resultoo in a further increase in production. Coai cannot be usOO because it softens during heating and renders the charge impermeable. Coai mining was also unsafe because of the natural gas explosions until Humphry Davy introduced the miner's safety lamp and a great effort was ne00oo to pump out the water flooding Lhe mines. Using coai also solvoo the problem of cutting trees from the forests which were needed to build ships.
Pig iron containing 3-5% carbon is hard and brittle. It was u500 for making pots and pans, firegrates, some machine parts especially for steam engines, anchors, cannons and cannon balls. This was particularly important in warfare, because before the arrival of pig iron, cannons were made of bronze or brass which were more expensive. A small amount of pig iron was made into wrought iron (Figure 3). Wrought iron contains less than I% carbon is soft and malleable. 1t was usOO for the production of nails, small arms , agricultura! implements, horseshoes, wire, locks, and bolts.
CASTRJN (pi~ iron)
a:K' FlON (R;
CA'lT STEEL (HUNTSMAN 1740)
CAST Sltfl (CORT 17~JI Minor producl
Figure 3 - The First Industrial Revo1ution (1709): Production of cast iron in a coke blast
furnace and the different varieties of steel.
Once the blast furnace technology using coke was established, efforts were made to economize its consumption and to cope with increased productivity .
ln 1828, the Scots engineer James B. Neilson (1792-1865) provosed preheating the ai r blast to about 95"C by passing the cold blast in a stove heated by burning coai. This decreased coke consumption by half and doubled pig iron prod uction .
ln 1845, Edward Cowper burned blast furnace gas in the stoves to supply the heat instead of burning coai . However, to collect the gas it was necessary first to design a device to close the top of the furnace . Thus carne the single-bell top into existence followed by the double-bell to eliminate complete1y the escape of gases .
ln some plants the blast furnace gas was first used to generate steam in a boilcr before being burned in the stoves. Steam was used in the steam engine to blow air in the tuyeres (Figure 3).
ln 1900 the casting machine was introduced to rep1ace the sand moulds in the ground. This became necessary due to increased furnace production . The molten iron was poured into the moulds from a !adie and cooled by water sprays as the chain travei to Lhe head sprocket, falling from the mould into wagons.
Many improvements were !ater introduced to economize fuel, e.g . , sizi:,g c the charge, air preheating to 1000C, etc.
Many improvements were !ater introduced to economize fuel, e.g., sizing of the charge, air preheating to lOO
MILOSTEEL (Bessemer 1856)
cx:N: IRCl'l CH:
MILOSTEEL (Siemens-Martin 1863)
Figure 4 - The Second Industrial Revolution (1856): The Bessemer converter.
Bottom-blown converter. The bottom-blown converter invented in Canada and Germany in 1970's in which oxygen was introduced at the bottom of the reactor. lt was evident for a long time that bottom-blowing is more efficient than top-blowing (better agitation, less dust formation, less noise, etc.), but no material of construction was available that can withstand the high temperature generated at the tuyeres when oxygen was used. The solution was found when the tuyeres were enveloped by a small stream of natural gas. The cracking of the hydrocarbons cooled the tips of the tuyeres and prevented their melting.
Top-blown bottom-blown steel. Today, ali primary steel is produced by a simultaneous top-blowing and bottom-blowing using oxygen, which results in higher productivity in a shorter time. ln addition continuous casting of steel started in 1960's became today the major technology (Figure 5).
::!1 o z o i= o ::;)
8 a: 0..
Figure 5 - Changing technology in steel production.
While organic chemistry is the chemistry of carbon, ferrous metallurgy is lhe technology of carbon. The carbon first used was charcoal produced from timber. When coai mining became safe, attempts were made to replace charcoal by coai, until lhe solution was found by first transforming coai into coke. Coke was first produced by piling coai in mounds and partially buming it in the open air in the sarne way charcoal was made.
The beehive process. Beehive ovens replaced lhe open air melhod in 1763. The volatile matter was bumed to supply heat for carbonization.
The horizontal retons process. The first attempt to recover lhe volatile matter was in the horizontal retorts system. The gas collected was known as coal-gas and was